1 Component: SC /10 SikaTop 144 DIVISION 7-THERMAL & MOISTURE PROTECTION Section Cementitious & Reactive Waterproofing DIVISION 9 - FINISHES Section Protective Coatings Part 1 General 1.01 Summary A. This specification describes the coating of substrates with a non-vapor barrier, protective dampproofing, waterproofing, polymer-modified, portland cement slurry Quality Assurance A. Manufacturing qualifications: The manufacturer of the specified product shall be ISO 9001 certified and have in existence a recognized ongoing quality assurance program independently audited on a regular basis. B. Contractor qualifications: Contractor shall be qualified in the field of concrete repair and protection with a successful track record of 5 years or more. Contractor shall maintain qualified personnel who have receivced product training by manufacturer's representative C. Install materials in accordance with all safety and weather conditions required by manufacturer or as modified by applicable rules and regulations of local, state and federal authorities having jurisdiction. Consult Material Safety Data Sheets for complete handling recommendations Delivery, Storage, and Handling A. All materials must be delivered in original, unopened containers with the manufacturer's name, labels, product identification, and batch numbers. Damaged material must be removed from the site immediately. B. Store all materials off the ground and protect from rain, freezing or excessive heat until ready for use. C. Condition the specified product as recommended by the manufacturer Job Conditions A. Environmental Conditions: Do not apply material if it is raining or snowing or if such conditions appear to be imminent. Minimum application temperature 45ºF (5ºC) and rising. B. Protection: Precautions should be taken to avoid damage to any surface near the work zone due to mixing and handling of the specified material Submittals A. Submit two copies of manufacturer's literature, to include: Product Data Sheets, and appropriate Material Safety Data Sheets (MSDS). B. Submit copy of Certificate of Approved Contractor status by manufacturer Warranty A. Provide a written warranty from the manufacturer against defects of materials for a period of one (1) year, beginning with date of substantial completion of the project.
2 Part 2 - Products 2.01 Manufacturer A. SikaTop 144, as manufactured by Sika Corporation, is considered to conform to the requirements of this specification Materials A. Polymer-modified portland cement coating: 2.03 Performance Criteria Component A shall be a liquid polymer emulsion of an acrylic co-polymer base and additives. Component B shall be a blend of selected portlandcements, specially graded aggregates, and admixtures to control setting time and workablity. The ratio of Componet A: Component B shall be: Mortar 1:1.647 by wieght The material shall be non-combustible, either before or after cure. A. Properties of the mixed polymer-modified portland cement coating:: 1. Pot Life: Approx. 4 hours 2. Color: gray or white 3. Recoat Time: 2 hours minimum between coats 4. Application thickness: 8-16 mils/ coat B. Properties of the cured polymer-modified portland cement coating: 1. Bond Strength (ACI 503R-30 Modified): Pull-off test 7 days - concrete substrate failure 2. Moisture Vapor permeability (ASTM E96) 7 days 1 coat 27 grains/hr./ft 2 2 coats 24 grains/hr./ft 2 4. Abrasion Resistance (ASTM D-968 Modified) 7 days 55liters/mil 5. The material shall not produce a vapor barrier. 6. The material shall be thermally compatible with portland cement mortar and concrete. 7. The material shall be approved by the United Staes Department of Agriculture. Note: Tests above were performed with the material and curing 71 o F 75 o F and 45-55%relative humidity.
3 Part 3 Execution 3.01 Surface Preparation A. Substrate must be clean, sound, and free of surface contaminants. Remove dust, laitance, grease, oils, curing compounds, form release agents and all foreign particles by mechanical means. An open-textured, sandpaper-like substrate is ideal. Substrate shall be in accordance with ICRI Guideline No for coatings and fall within CSP4. All surfaces must be saturated surface dry (SSD), with no standing water at time of application Mixing and Application A. Mixing: Under normal circumstances, full quantities of both components are mixed together, a slurry consistency will result. Mix in a clean container by slowly adding the powder component to the liquid component and mixing with a slow speed ( rpm) drill and mixing paddle. B. Coating Application: Apply with stiff bristle brush, roller, or spray equipment. Work material into the prepared substrates, filling all pores and voids. For brush grade: Apply first coat, with horizontal brush strokes and leave to harden (2 to 4 hours). Apply second coat with vertical brush stokes. For spray application: Use a hopper gun spray equipment, textured sprayer (e.g. Texspray E110c by Graco), or a rotor/stator pump equipment. Allow the first coat to harden (2 to 4 hours) prior to the application of the second coat. As soon as the second coat is applied an optional back roller to get desired appearance. C. When applying the coating, never stop the application until the entire surface has been coated. Always stop application at an edge, corner, or joint. Never let a previously coated film dry; always coat into a wet film. Always apply the coating at a 45 o angle to an edge, corner, or joint. D. Adhere to all limitations and cautions for the polymer-modified cement coating in the manufacturer's printed literature Cleaning A. The uncured polmer-modified portland cement coating can be cleaned from tools with water. The cured polymermodified portland cement coating coating can only be removed mechanically. B. Leave finished work and work area in a neat, clean condition without evidence of spillovers onto adjacent areas.
4 SC-057 SikaTop 144 Surface Coating 1. Substrate surface preparation shall provide a clean and sound surface with a finish profile of a CSP-1 to 3 as per ICRI Technical Guidlines 2. Pre-soak to provide saturated surface dry (SSD) substrate condition prior to applying coating material. 3. Apply 2-coats of SikaTop Seal 144 with a stiff bristled brush, broom, or hopper type spray equipment. (milage thickness per technical data sheet) Concrete Restoration Systems by Sika Corporation, 201 Polito Avenue, Lyndhurst, NJ SIKA CORPORATION MAKES NO WARRANTY OF ANY KIND, EITHER EXPRESS OR IMPLIED, AS TO THE ACCURACY, COMPLETENESS OR THE CONTENTS OF THESE GUIDE SPECIFICATIONS SIKA SHALL NOT BE RESPONSIBLE UNDER ANY LEGAL THEORY TO ANY THIRD PARTY FOR ANY DIRECT OR CONSEQUENTIAL DAMAGES OF ANY KIND ARISING FROM THE USE OF THESE GUIDE SPECIFICATIONS.
5 Prior to each use of any Sika product, the user must always read and follow the warnings and instructions on the product's most current Technical Data Sheet, product label and Material Safety Data Sheet which are available at or by calling (201) Nothing contained in any Sika materials relieves the user of the obligation to read and follow the warnings and instructions for each Sika product as set forth in the current Technical Data Sheet, product label and Material Safety Data Sheet prior to product use.